#------------------------------------------------------------------------------
#$Date: 2014-08-15 21:12:14 +0300 (Fri, 15 Aug 2014) $
#$Revision: 22 $
#$URL: svn+ssh://sauliusg@svn.code.sf.net/p/propcif/code/trunk/cif/1/1000051.mpod $
#------------------------------------------------------------------------------
#
# This file is available in the Material Properties Open Database (MPOD),
# http://www.mpod.net/
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_1000051
_cod_database_code               ?
_structure_refined 'no'
_mpod_phase_name Pb(Zn1/3Nb2/3)O3-PbTiO3(0.07)
_chemical_formula_sum 'Pb Nb0.62 Zn0.31 Ti0.07 O3'
_mpod_phase_generic_name 'PZN-PT'
_mpod_symmetry_point_group_name_H-M 3m
_cell_length_a  ?
_cell_length_c  ?
loop_
_publ_author_name
'Zhang R.'
'Jiang B.' 
'Jiang W.'
'Cao W.'
_publ_section_title
;
Complete set of elastic, dielectric, and piezoelectric coefficients of 0.93Pb(Zn1/3Nb2/3)O3-0.07PbTiO3 single crystal poled along [011]
;
_journal_name_full               'Applied Physics Letters'
_journal_volume                  89
_journal_issue                   24
_journal_article_reference       242908
_journal_pages_number             3
_journal_year                    2006
_mpod_phase_density 8038.4
_mpod_phase_transition_temperature_rhomb_tetra ?
_mpod_phase_transition_temperature_curie ?
_prop_measurement_poling '[011]c'
_prop_symmetry_point_group_name_H-M mm2
_prop_frame '1=[0-11]c 2=[100]c 3=[011]c'
_prop_elastic_compliance_sijD 'sijD'
_prop_elastic_compliance_sijE 'sijE'
_prop_elastic_stiffness_cijD 'cijD'
_prop_elastic_stiffness_cijE 'cijE'
_prop_electromechanical_coupling_kij 'kij'
_prop_piezoelectric_dij 'dij'
_prop_piezoelectric_eij 'eij'
_prop_piezoelectric_gij 'gij'
_prop_piezoelectric_hij 'hij'
_prop_dielectric_permittivity_relative_epsrijT 'epsrijT'
_prop_dielectric_stiffness_relative_betrijT 'betrijT'
_prop_dielectric_permittivity_relative_epsrijS 'epsrijS'
_prop_dielectric_stiffness_relative_betrijS 'betrijS'
loop_
_prop_data_label
_prop_data_tensorial_index
_prop_data_value
_prop_measurement_method
_prop_conditions_frequency
cijE 11 145 'RUS' ?
cijE 12 153.16 'RUS' ?
cijE 13 126.66 'RUS' ?
cijE 22 180.24 'RUS' ?
cijE 23 150 'RUS' ?
cijE 33 141 'RUS' ?
cijE 44 64.72 'RUS' ?
cijE 55 34.3 'RUS' ?
cijE 66 71 'RUS' ?
cijD 11 173.987 'RUS' ?
cijD 12 211.639 'RUS' ?
cijD 13 114.275 'RUS' ?
cijD 22 180.240 'RUS' ?
cijD 23 125.014 'RUS' ?
cijD 33 146.292 'RUS' ?
cijD 44 65.360 'RUS' ?
cijD 55 40.65 'RUS' ?
cijD 66 71.000 'RUS' ?
sijE 11 67.5153 'RUS' ?
sijE 12 -60.1637 'RUS' ?
sijE 13 3.3551 'RUS' ?
sijE 22 102.0024 'RUS' ?
sijE 23 -54.4683 'RUS' ?
sijE 33 62.0233 'RUS' ?
sijE 44 15.4512 'RUS' ?
sijE 55 291.5452 'RUS' ?
sijE 66 14.0845 'RUS' ?
sijD 11 59.4003 'RUS' ?
sijD 12 -35.3773 'RUS' ?
sijD 13 -16.1684 'RUS' ?
sijD 22 26.2949 'RUS' ?
sijD 23 5.1644 'RUS' ?
sijD 33 15.0523 'RUS' ?
sijD 44 15.2998 'RUS' ?
sijD 55 245.9933 'RUS' ?
sijD 66 14.0845 'RUS' ?
dij 15 1823 'RUS' ?
dij 24 50 'RUS' ?
dij 31 478 'RUS' ?
dij 32 -1460 'RUS' ?
dij 33 1150 'RUS' ?
eij 15 6.2529 'RUS' ?
eij 24 3.2360 'RUS' ?
eij 31 -8.6446 'RUS' ?
eij 32 -17.4399 'RUS' ?
eij 33 3.6935 'RUS' ?
gij 15 2.49873 'RUS' ?
gij 24 0.30280 'RUS' ?
gij 31 1.69770 'RUS' ?
gij 32 -5.18545 'RUS' ?
gij 33 4.08443 'RUS' ?
hij 15 1.0158 'RUS' ?
hij 24 1.9791 'RUS' ?
hij 31 -33.5315 'RUS' ?
hij 32 -67.6476 'RUS' ?
hij 33 14.3266 'RUS' ?
kij 15 0.4 'RUS' ?
kij 24 0.1 'RUS' ?
kij 31 0.35 'RUS' ?
kij 32 0.86 'RUS' ?
kij 33 0.87 'RUS' ?
epsrijT 11 8240 'CAP' 1
epsrijT 22 1865 'CAP' 1
epsrijT 33 3180 'CAP' 1
betrijT 11 1.2136 'CAP' 1
betrijT 22 5.3619 'CAP' 1
betrijT 33 3.1440 'CAP' 1
epsrijS 11 6953 'CAP' 10000
epsrijS 22 1847 'CAP' 10000
epsrijS 33 291 'CAP' 10000
betrijS 11 1.4383 'CAP' 10000
betrijS 22 5.4150 'CAP' 10000
betrijS 33 34.3440 'CAP' 10000
